Research Article Electrospun Carbon Nanofiber Membranes ... Article Electrospun Carbon Nanofiber...
Embed Size (px)
Transcript of Research Article Electrospun Carbon Nanofiber Membranes ... Article Electrospun Carbon Nanofiber...
Research ArticleElectrospun Carbon Nanofiber Membranes forFiltration of Nanoparticles from Water
Mirko Faccini, Guadalupe Borja, Marcel Boerrigter,Diego Morillo Martn, Sandra Martnez Crespiera, Socorro Vzquez-Campos,Laurent Aubouy, and David Amantia
LEITAT Technological Center, C/de la Innovacio 2, 08225 Terrassa, Spain
Correspondence should be addressed to Mirko Faccini; email@example.com
Received 13 October 2014; Accepted 12 December 2014
Academic Editor: Fujuan Liu
Copyright 2015 Mirko Faccini et al. This is an open access article distributed under the Creative Commons Attribution License,which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Nowadays, hundreds of consumer products contain metal and metal oxide nanoparticles (NP); this increases the probabilityof such particles to be released to natural waters generating a potential risk to human health and the environment. This paperpresents the development of efficient carboneous nanofibrous membranes for NP filtration from aqueous solutions. Free-standingcarbon nanofiber (CNF) mats with different fiber size distribution ranging from 126 to 554 nm in diameter were produced byelectrospinning of polyacrylonitrile (PAN) precursor solution followed by thermal treatment. Moreover, tetraethoxyorthosilicatewas added to provide flexibility and increase the specific surface area of the CNF. The resulting membranes are bendable andmechanically strong enough to withstand filtration under pressure or vacuum. The experimental results of filtration revealed thatthe fabricated membranes could efficiently reject nanoparticles of different types (Au, Ag, and TiO
2) and size (from 10 to 100 nm
in diameter) from aqueous solutions. It is worth mentioning that the removal of Ag NP with diameters as small as 10 nm was closeto 100% with an extremely high flux of 47620 Lm2 h1 bar1.
Nanotechnology is having a large impact in manufacturedproducts in most major industry sectors, including elec-tronic, cosmetic, automotive, and healthcare sectors. Accord-ing to a recent survey  over 1,300 nanotechnology-relatedproducts are currently on the market. Free nanoparticles(NP) are likely to enter the aquatic environment in all stagesof nanomaterials life cycle (production, processing, use,recycling, and disposal).These particles can persist in naturalbodies and are not fully removed by drinkingwater treatmentsystems, thereby posing a potential public health concern[2, 3]. Therefore, the development of new barrier materialsis needed to reduce the potential risks related to humanand environmental exposure to nanomaterials . Nanofiberwebs, due to their very large specific area, very small poresize, and high porosity, have been shown to improve theefficiency of conventionalmaterials used for the filtration andseparation of particulate materials [5, 6].
Electrospinning is a well-established and versatile processthat has been used to produce ultrafine fibers includingmicrofibers (>1 m) or nanofibers (
2 Journal of Nanomaterials
membranes were fabricated by electrospinning of a poly-acrylonitrile (PAN) precursor solution followed by a thermaltreatment of the electrospun fibers. Moreover, tetraethoxy-orthosilicate (TEOS) was added to provide flexibility and toincrease the specific surface area of the CNF [13, 14].
To the best of our knowledge, CNF derived fromPAN/TEOS have not been used for such filtration purposes.Unlike carbonized PAN mats, which were too brittle to tol-erate high vacuum filtration process, the PAN/TEOS derivedCNF mats were bendable and showed sufficient mechanicalstrength to withstand filtration under pressure or vacuum.The experimental results demonstrate that the membranescould efficiently reject various NP (Au, Ag, and TiO
different sizes and natures from the aqueous solution.
2. Experimental Part
2.1.Materials andMethods. PAN (Mw= 150,000 g/mol) pow-der, N-N dimethylformamide (DMF), and TEOS (98%) werepurchased from Sigma-Aldrich. CNF precursor solutionswere prepared by dissolving PAN at concentrations rangingfrom 4 to 12 wt.% in DMF at 60C. PAN/TEOS precursorsolutions were prepared by the addition of TEOS to thePAN solutions in DMF to achieve the proper PAN/TEOSweight ratios, as shown in Table 2. All polymer solutionswere mixed by a magnetic stirrer for a sufficiently long timeuntil they became homogeneous. The viscosity and electricalconductivity of polymer solutions were measured by a digitalviscometer (DV-E, Brookfield Co.) and an electric conduc-tivity meter (CRISON EC-meter BASIC) at 25C. To producenanofibers the solutions were electrospun onto an aluminumfoil by using commercially available electrospinning equip-ment (MECCCo. LTD.,modelNF-103). Plastic syringes fittedwith metal needles were used as electrospinning nozzles.Typical operating conditions were the following: flow rates of1-2mL/h, applied voltages between 25 and 30 kV, andworkingdistance of 916 cm. For carbonization, the as-spun polymerfibers were first placed in a chamber furnace and stabilizedin air for 5 hours at 280C and then carbonized for 1 hourin nitrogen at 8001000C; in both cases the ramp rate was1C/min .
2.2. Preparation of the NP Solutions. The filtration perfor-mance of carbonized PAN/TEOS nanofibers was evaluatedwith different types of NP, including metallic NP, such as Agand Au, and metal oxide NP, such as TiO
were prepared by the sonication of proper amounts of NP inmilliQ water for 10min at 50% of the total power (750W).Au and Ag aqueous nanoparticle solutions were kindlyprovided by ICN (Catalonia Institute of Nanotechnology).The concentrations of the NP solutions were adjusted to havea high ultraviolet-visible (UV-vis) absorbance without signalsaturation.
2.3. Characterization. The surface morphology of the nano-fibermats was examined using scanning electronmicroscopy(SEM, Zeiss Evo MA-10) after coating with carbon to min-imize the charging effect. Images taken by the SEM were
analyzed to obtain the fiber diameter by the ImageJ software.At least four pictures were used to calculate the mean valuesof the diameter of the fibers.
The clean water permeance (CWP) of CNF membraneswas determined using a bench-scale dead-end filtrationsetup. The system consists of a reservoir tank containingultrapure water (Type 1) connected to a 200mL Amiconstirred ultrafiltration cell (Merck Millipore). The stirred cellhouses a 63.5mm diameter flat CNF sheet with an effectivearea of 28.7 cm2. Pressure in the feed tank was provided bycompressed air. The applied pressure measured during theCWP experiments was 3 kPa (0.43 psi).
The pore size of the CNF membranes was determinedusing a simple particle removalmethod. Solutions containing20mg/L of polystyrene latex beads (from Magsphere Corp.)with diameter between 0.1 m and 3 mwere passed throughthemembrane at the pressure of about 0.1 bar.The absorbanceof the feed and filtrate latex solutions was measured usingUV-vis spectrometer and the removal rate was calculatedby the following formula, where feed and filtrate are theabsorbance at 250 nm of feed and filtrate solutions, respec-tively:
Removal rate% = [1 [ feedfiltrate]] 100. (1)
A latex removal curve was drawn by plotting the removalrates against the beads diameter size (Figure 7). The nominalpore size is defined as the diameter where 90% of latex beadsare removed.
For filtration experiments, disc filter was cut out of thenanofibrous mats by using a hollow punch and placed onthe metallic support of the filtration setup. A solution ofnanoparticles was passed through it andUV-vis spectrometerwas used to measure the absorbance of the feed and filtratesolutions. The filtration efficiency was calculated using thefollowing formula, where feed andfiltrate are the absorbanceat max of feed and filtrate solutions, respectively:
Filtration efficiency% = [[ feed filtrate]
feed] 100. (2)
3. Result and Discussion
3.1. CNF Membranes. It is known that the morphology ofelectrospun fibers depends on various processing parameters,solution properties, and environmental conditions. Throughcontrol of the spinning conditions, the resulting fibers canrange fromabout 20 nm to a fewmicrometers. To gain controlover the properties of the obtained nanofibers, the viscosityand conductivity were measured as a function of the PANconcentration. Figure 1 shows an overlay plot of the viscosityand conductivity as function of the PAN weight percentagein DMF. By increasing the PAN concentration from 4 to12wt.% the viscosity rises exponentially from 31 to 2053 cP,as a result of the higher molecular entanglement. In fact, athigher precursor concentration the polymer chains are moretangled, which leads to the production of broader fibers. Theelectric conductivity also increases from 48 to 86 s/cm by
Journal of Nanomaterials 3
Table 1: Process parameters used for the electrospinning of solutions C-1 to C-5 and the average diameters of the PAN nanofibers and CNFmats.
Solution code PAN Feed rate Voltage Distance Applied electric field PAN nanofibers diameter Carbon nanofibers diameter(wt.%) (mL/h) (kV) (cm) (kV/cm) (nm) (nm)
C-1 4 2 30 7 4.2 96 24 C-2 6 2 30 10 3.0 189 47 126 19C-3 8 2 29 13 2.2 282 51 184 31C-4 10 2 29 15 1.9 351 78 249 24C-5 12 2 27 16 1.7 620 39 554 107
Table 2: Characterization of the PAN/TEOS solutions C-Si-1 to C-Si-3 and the average diameters of the PAN/TEOS nanofibers and CNF/Simats.
Solution code PAN PAN/TEOS Viscosity Conductivity PAN/TEOS nanofibers diameter CNF/Si diameter(wt.%) (w/w) (cP) (s/cm) (nm) (nm)
C-Si-1 6 7/3 132 96 244 31 158 38C-Si-2 8 7/3 285 93 300 33 193 36C-Si-3 10 7/3 647 102 487 65 387 33